Tuning of Charge Transfer Assisted Phase Transition and Slow Magnetic Relaxation Functionalities in {Fe(9-x)Co(x)[W(CN)8]6} (x = 0-9) Molecular Solid Solution.
Chorazy, Szymon; Stanek, Jan J.; Nogaś, Wojciech; Majcher, Anna M.; Rams, Michał; Kozieł, Marcin; Juszyńska-Gałązka, Ewa; Nakabayashi, Koji; Ohkoshi, Shin-ichi; Sieklucka, Barbara; Podgajny, Robert; Journal of the American Chemical Society 138 (2016) 1635–1646; doi:10.1021/jacs.5b11924

data_4129915
_publ_section_title
;
 Tuning of Charge Transfer Assisted Phase Transition and Slow Magnetic
 Relaxation Functionalities in {Fe(9-x)Co(x)[W(CN)8]6} (x = 0-9) Molecular
 Solid Solution.
;
_journal_issue                   5
_journal_name_full               'Journal of the American Chemical Society'
_journal_page_first              1635
_journal_page_last               1646
_journal_paper_doi               10.1021/jacs.5b11924
_journal_volume                  138
_journal_year                    2016
_chemical_formula_moiety         'C84 H60 Co Fe8 N48 O36 W6'
_chemical_formula_sum            'C84 H60 Co Fe8 N48 O36 W6'
_chemical_formula_weight         3926.63
_space_group_IT_number           15
_space_group_name_Hall           '-C 2yc'
_space_group_name_H-M_alt        'C 1 2/c 1'
_symmetry_cell_setting           monoclinic
_symmetry_Int_Tables_number      15
_symmetry_space_group_name_Hall  '-C 2yc'
_symmetry_space_group_name_H-M   'C 1 2/c 1'
_atom_sites_solution_hydrogens   geom
_audit_conform_dict_location     ftp://ftp.iucr.org/pub/cif_core.dic
_audit_conform_dict_name         cif_core.dic
_audit_conform_dict_version      2.4.3
_audit_creation_date             2015-01-26T16:54:01-00:00
_audit_creation_method           'WinGX routine CIF_UPDATE'
_cell_angle_alpha                90
_cell_angle_beta                 114.6080(10)
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   28.6522(13)
_cell_length_b                   18.7712(7)
_cell_length_c                   32.1509(15)
_cell_measurement_reflns_used    72385
_cell_measurement_temperature    130(2)
_cell_measurement_theta_max      27.459
_cell_measurement_theta_min      3.001
_cell_measurement_wavelength     0.71075
_cell_volume                     15721.4(12)
_computing_molecular_graphics    'Ortep for Windows (Farrugia, 2012)'
_computing_publication_material  'WinGX publication routines (Farrugia, 2012)'
_computing_structure_refinement  'SHELXL-2014/7 (Sheldrick, 2014)'
_diffrn_ambient_temperature      130(2)
_diffrn_measured_fraction_theta_full 0.994
_diffrn_measured_fraction_theta_max 0.988
_diffrn_measurement_device_type  'Rigaku R-AXIS RAPID'
_diffrn_measurement_method       \w
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71075
_diffrn_reflns_av_R_equivalents  0.0652
_diffrn_reflns_av_unetI/netI     0.054
_diffrn_reflns_Laue_measured_fraction_full 0.994
_diffrn_reflns_Laue_measured_fraction_max 0.988
_diffrn_reflns_limit_h_max       36
_diffrn_reflns_limit_h_min       -37
_diffrn_reflns_limit_k_max       24
_diffrn_reflns_limit_k_min       -24
_diffrn_reflns_limit_l_max       41
_diffrn_reflns_limit_l_min       -37
_diffrn_reflns_number            72385
_diffrn_reflns_point_group_measured_fraction_full 0.994
_diffrn_reflns_point_group_measured_fraction_max 0.988
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         27.459
_diffrn_reflns_theta_min         3.001
_diffrn_standards_number         0
_exptl_absorpt_coefficient_mu    5.258
_exptl_absorpt_correction_T_max  0.591
_exptl_absorpt_correction_T_min  0.445
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   'ABSCOR (Rigaku, 1995)'
_exptl_crystal_colour            green
_exptl_crystal_density_diffrn    1.659
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       block
_exptl_crystal_F_000             7468
_exptl_crystal_size_max          0.2
_exptl_crystal_size_mid          0.13
_exptl_crystal_size_min          0.1
_refine_diff_density_max         2.867
_refine_diff_density_min         -2.544
_refine_diff_density_rms         0.19
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.043
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_constraints    0
_refine_ls_number_parameters     849
_refine_ls_number_reflns         17781
_refine_ls_number_restraints     80
_refine_ls_restrained_S_all      1.046
_refine_ls_R_factor_all          0.08
_refine_ls_R_factor_gt           0.0594
_refine_ls_shift/su_max          0.026
_refine_ls_shift/su_mean         0
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[\s^2^(Fo^2^)+(0.0539P)^2^+287.9720P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1318
_refine_ls_wR_factor_ref         0.1426
_reflns_Friedel_coverage         0
_reflns_number_gt                13949
_reflns_number_total             17781
_reflns_threshold_expression     'I > 2\s(I)'
_cod_data_source_file            ja5b11924_si_003.cif
_cod_data_source_block           Co1Fe8W6_LT
_cod_original_sg_symbol_H-M      'C 2/c'
_cod_database_code               4129915
_shelx_estimated_absorpt_t_min   0.419
_shelx_estimated_absorpt_t_max   0.621